**50th anniversary of JTAM**

**THE INFLUENCE OF MATERIAL PROPERTIES AND CRACK**
**LENGTH ON THE Q-STRESS VALUE NEAR THE CRACK TIP**

**FOR ELASTIC-PLASTIC MATERIALS FOR CENTRALLY**
**CRACKED PLATE IN TENSION**

Marcin Graba

*Kielce University of Technology, Faculty of Mechatronics and Machine Design, Kielce, Poland*
*e-mail: [email protected]*

*In the paper, values of the Q-stress determined for various elastic-plastic*
materials for centre cracked plate in tension (CC(T)) are presented. The
inﬂuence of the yield strength, the work-hardening exponent and the
*crack length on the Q-parameter was tested. The numerical results were*
approximated by closed form formulas. This paper is a continuation of
the catalogue of the numerical solutions presented in 2008, which
*pre-sents Q-stress solutions for single edge notch specimens in bending –*
SEN(B). Both papers present full numerical results and their
approxi-mation for two basic specimens which are used to determine in the
*labo-ratory tests the fracture toughness – J-integral, and both specimens are*
proposed by FITNET procedure used to idealize the real components.

*Key words: fracture mechanics, cracks, Q-stress, stress ﬁelds, HRR *

*so-lution, FEM, J-integral, O’Dowd theory*

**1.** * Introduction – theoretical backgrounds about J-Q theory*
The stress ﬁeld near crack tip for the non-linear Ramberg-Osgood (R-O)
mate-rial was described in 1968 by Hutchinsonson, who published the fundamental
work for fracture mechanics. The presented by Hutchinson solution, now
cal-led “the HRR solution”, includes the ﬁrst term of the inﬁnite series only. The
numerical analysis shows that the results obtained using the HRR solution
are diﬀerent from the results obtained using the ﬁnite element method – FEM
(Fig. 1). To eliminate this diﬀerence, it is necessary to use more terms in the
HRR solution.

Fig. 1. Comparison of FEM results and HRR solution for the plane stress and plane strain for a single edge notched specimen in bending (SEN(B)) and centrally cracked

*plate in tension (CC(T)); E = 206000 MPa, n = 5, ν = 0.3, σ*0= 315 MPa,
*ε*0*= σ*0*/E = 0.00153, a/W = 0.50, W = 40 mm, θ = 0*

First it was done by Li and Wang (1985), who using two terms in the
Airy function, obtained the second term of the asymptotic expansion only
*for two diﬀerent materials, described by the R-O exponent equal to n = 3*
*and n = 10. Their analysis shows that the two term solution much better*
describes the stress ﬁeld near the crack tip, and the value of the second term,
which may not to be negligible depends on the material properties and the
specimen geometry.

*A more accurate solution was proposed by Yang et al. (1993), who using the*
Airy function with the separate variables proposed that the stress ﬁeld near the
crack tip may be described by an inﬁnite series form. The proposed by them
solution is currently used with only three terms of the asymptotic solution, and
*it is often called “J-A2* *theory”. Yang et al. (1993) conducted full discussion*
about their idea. They showed that the multi-terms description, which uses
three terms of the asymptotic solution is better than the Hutchinson approach.
*The A2* *amplitude, which is used in the J-A2* *theory suggested by Yang et al.*
(1993) is nearly independent of the distance of the determination, but using the

*J-A*2 theory in engineering practice is sometimes very burdensome, because
an engineer must know the *σ*e_{ij}(k)*function and the power exponent t, which*
are to be calculated by solving a fourth order diﬀerential equation, and next
*using FEM results, the engineer must calculate the A*2 amplitude.

The simpliﬁed solution for describing the stress ﬁeld near the crack tip
for elastic plastic materials was proposed by O’Dowd and Shih (1991, 1992).
*That concept was discussed by Shih et al. (1993). They assumed that the FEM*
results are exact and computed the diﬀerence between the numerical and HRR

results. They proposed that the stress ﬁeld near the crack tip may be described by the following equation

*σij* *= σ*0
_{J}*αε*0*σ*0*In(n)r*
1
*n*+1
e
*σij(θ, n) + σ*0*Q*
_{r}*J/σ*0
*q*
b
*σij(θ, n)* (1.1)

*where r and θ are polar coordinates of the coordinate system located at the*
*crack tip, σij* *are the components of the stress tensor, J is the J-integral, n is*

*the R-O exponent, α is the R-O constant, σ*0 *– the yield stress, ε*0 – strain
*related to σ*0*through ε*0*= σ*0*/E,* *σ*b*ij(θ; n) are functions evaluated *

*numerical-ly, q is the power exponent whose value changes in the range (0;0.071), and*

*Q is a parameter, which is the amplitude of the second term in the asymptotic*

solution. The functions *σ*e*ij(n, θ), In(n) must be found by solving the fourth*

order non-linear homogenous diﬀerential equation independently for the plane stress and plane strain (Hutchinson, 1968) or these functions may be found using the algorithm and computer code presented in Gałkiewicz and Graba (2006).

*O’Dowd and Shih (1991, 1992) tested the Q-parameter in the range*

*J/σ*0 *< r < 5J/σ*0 *near the crack tip. They showed, that the Q-parameter*
*weakly depends on the crack tip distance in the range of ±π/2. They proposed*
only two terms to describe the stress ﬁeld near the crack tip

*σij* *= (σij*)*HRR+ Qσ0σ*b*ij(θ)* (1.2)

*where (σij*)*HRR*( is the ﬁrst term of Eq. (1.1) and it is the HRR solution.

*To avoid the ambiguity during the calculation of the Q-stress, O’Dowd*
*and Shih (1991, 1992) suggested that the Q-stress should be computed at*
*the distance from the crack tip which is equal to r = 2J/σ*0 for the direction

*θ = 0. They postulated that for the θ = 0 direction the function* *σ*b*θθ(θ = 0)*

*is equal to 1. That is why the Q-stress may be calculated from the following*
relationship

*Q =* *(σθθ*)*F EM* *− (σθθ*)*HRR*
*σ*0

*for θ = 0* and *rσ*0

*J* = 2 (1.3)

*where (σθθ*)*F EM* *is the stress value calculated using FEM and (σθθ*)*HRR* is the

stress evaluated form the HRR solution (these are the opening crack tip stress components).

*During analysis, O’Dowd and Shih (1991, 1992) showed that the Q-stress*
value determines the level of the hydrostatic stress. For a plane stress, the

*Q-parameter is equal to zero or it is close to zero, but for a plane strain, the*
*Q-parameter is in the most cases smaller than zero (Fig. 2). The Q-stress value*

for a plane strain depends on the external loading and distance from the crack tip – especially for large external loads (Fig. 2b).

*Fig. 2. J-Q trajectories measured at six distances near the crack tip for centrally*
cracked plate in tension (CC(T)): (a) plane stress, (b) plane strain (own calculation);

*W = 40 mm, a/W = 0.5, σ*0*= 315 MPa, ν = 0.3, E = 206000 MPa, n = 5*

**2.** **Engineering aspects of J-Q theory, fracture criteria based on****the O’Dowd approach**

Using the O’Dowd and Shih theory to describe the stress ﬁeld near the crack tip
for elastic-plastic materials, the diﬀerence between the HRR solution
(Hutch-nison, 1968) and the results obtained using the ﬁnite element method (FEM)
can be eliminated. O’Dowd’s theory is quite simple to use in practice, because
in order to describe the stress ﬁeld near the crack tip, we must know only
*ma-terial properties (yield stress, work hardening exponent), J-integral and the*

*Q-stress value, which may be evaluated numerically or determined using the*

approximation presented in literature, for example Graba (2008). O’Dowd’s
*approach is easier and more convenient to use in contrast to J-A*2 theory,
*which was proposed by Yang et al. (1993). Based on the J-Q theory, O’Dowd*
(1995) proposed the following fracture criterion

*JC* *= JIC*
*1 −* *Q*
*σc/σ*0
*n+1*
(2.1)
*where JC* is the real fracture toughness for a structural element characterised

*by a geometrical constraint deﬁned by Q-stress (whose value is usually is*
*smaller than zero), JIC* is the fracture toughness for the plane strain condition

*for Q = 0 and σc* is the critical stress according to the Ritchie-Knott-Rice

*hypothesis (Ritchie et al., 1973).*

*Proposed by O’Dowd fracture criterion was discussed by Neimitz et al.*
(2007), where the authors proposed another form. They modiﬁed O’Dowd’s

*formulas (Eq. (2.1)), by replacing the critical stress σc* by maximum opening

*stress σmax*, which must be evaluated numerically using the large strain

*for-mulation. The proposed by Neimitz et al. (2007) formulas have the following*
form
*JC* *= JIC*
*1 −* *Q*
*σmax/σ*0
*n+1*
(2.2)
*For a single edge notch in bending (SEN(B)), Neimitz et al. (2007) – using*
the ﬁnite element method and the large strain formulation – estimated the
*maximum opening stress σmax*for several materials (diﬀerent R-O exponents,

diﬀerent yield stresses) and for several crack lengths.

*The J-Q theory found application in European Engineering Programs, like*
*SINTAP (1999) or FITNET (2006). The Q-stresses are applied for *
construc-tion of the fracture criterion and to assess the fracture toughness of structural
*components. The real fracture toughness K _{mat}C* may be evaluated using the
formula proposed by Ainsworth and O’Dowd (1994). They showed that the
increase in fracture in both the brittle and ductile regimes may be represented
by an expression of the form

*K _{mat}C* =
(

*Kmat* *for βLr* *> 0*

*Kmat[1 + α(−βLr*)*k*] *for βLr* *< 0*

(2.3)
*where Kmat* is the fracture toughness for the plane strain condition obtained

*using FITNET procedures, and β is the parameter calculated using the *
follo-wing formula

*β =*

(

*T /(Lrσ*0) for elastic materials

*Q/Lr* for elastic-plastic materials

(2.4)
*where Lr* *is the ratio of the actual external load P and the limit load P*0
(or the reference stress), which may be calculated using FITNET procedures
(FITNET, 2006).

*The constants α and k, which are occurring in Eq. (2.3), are material and*
*temperature dependent (Table 1). Sherry et al. (2005a,b) proposed *
*procedu-res to calculate the constants α and k. Thus O’Dowd’s theory has practical*
application to engineering issues.

*Sometimes, the J-Q theory may be limited, because there is no value of the*

*Q-stress for a given material and specimen. Using any fracture criterion, for*

example that proposed by O’Dowd (1995) or another one, Eq. (2.3) (FITNET,
*2006) or that presented by Neimitz et al. (2007) (see Eq. (2.2)), or presented*
*by Neimitz et al. (2004), an engineer can estimate the fracture toughness quite*
*fast, if the Q-stress is known.*

* Table 1. Some values of the α and k parameters from Eq. (2.3) (SINTAP,*
1999; FITNET, 2006)

Material Temperature Fracture mode *α* *k*

A533B (steel) *−75◦*_{C} _{cleavage} _{1.0} _{1.0}

A533B (steel) *−90◦*_{C} _{cleavage} _{1.1} _{1.0}

A533B (steel) *−45◦*_{C} _{cleavage} _{1.3} _{1.0}

Low Carbon Steel *−50◦*_{C} _{cleavage} _{1.3} _{2.0}

A515 (steel) +20*◦*_{C} _{cleavage} _{1.5} _{1.0}

0.0 1.0

ASTM 710 Grade A +20*◦*_{C} _{ductile} _{0.6} _{1.0}

1.0 2.0

*Literature does not announce the Q-stress catalogue and Q-stress value as*
functions of the external load, material properties or geometry of the specimen.
*The numerical analysis shown in Graba (2008) indicates that the Q parameter*
depends on material properties, specimen geometry and external load. In some
*papers, an engineer may ﬁnd J-Q graphs for a certain group of materials. The*
*best solution will be the catalogue of J-Q graphs for materials characterised by*
various yield strengths, diﬀerent work-hardening exponents. Such a catalogue
should take into consideration the inﬂuence of the external load, kind of the
specimen (SEN(B) specimen – bending, CC(T) – tension or SEN(T) – tension)
and its geometry. For SEN(B) specimens, such a catalogue was presented in
*Graba (2008), who presented Q-stress values for specimens with predominance*
of bending for diﬀerent materials and crack lengths. In the literature, there
is no similar catalogue for specimens with predominance of tension. That is
*why, in the next parts of the paper, values of the Q-stress will be determined*
for various elastic-plastic materials for a centrally cracked plate in tension
(CC(T)). The CC(T) specimen is the basic structural element which is used in
the FITNET procedures (FITNET, 2006) to the modelling of real structures.
*All results will be presented in a graphical form – the Q = f (J) graphs. Next,*
the numerical results will be approximated by closed form formulas.

**3.** **Details of numerical analysis**

In the numerical analysis, the centrally cracked plate in tension (CC(T)) was
used (Fig. 3). Dimensions of the specimens satisfy the standard requirement
*which is set up in FEM calculation L 2W , where W is the width of the*
*specimen and L is the measuring length of the specimen. Computations were*

performed for a plane strain using small strain option. The relative crack
*length was a/W = {0.05, 0.20, 0.50, 0.70} where a is the crack length. The*
*width of specimens W was equal to 40 mm (for this case, the measuring length*

*L 80 mm). All geometrical dimensions of the CC(T) specimen are presented*

in Table 2.

Fig. 3. Centrally cracked plate in tension (CC(T))

**Table 2. Geometrical dimensions of the CC(T) specimen used in numerical**
analysis

width

*W*

[mm]

measuring total relative crack crack

length length length length

*4W [mm]* *2L [mm]* *a/W* *a [mm]*
40 160 176
0.05 2
0.20 8
0.50 20
0.70 28

The choice of the CC(T) specimen was intentional, because the CC(T)
specimens are used in the FITNET procedures (FITNET, 2006) for modelling
of real structural elements. Also in the FITNET procedures, the limit load
and stress intensity factors for CC(T) specimens are presented. However in
*the EPRI procedures (Kumar et al., 1981), the hybrid method for calculation*
*of the J-integral, crack opening displacement (COD) or crack tip opening*
displacement (CTOD) are given. Also some laboratory tests in order to
*de-termine the critical values of the J-integral may be done using the CC(T)*
specimen, see for example Sumpter and Forbes (1992).

Computations were performed using ADINA SYSTEM 8.4 (ADINA, 2006a,b). Due to the symmetry, only a quarter of the specimen was modelled. The ﬁnite element mesh was ﬁlled with 9-node plane strain elements. The size of the ﬁnite elements in the radial direction was decreasing towards the crack tip, while in the angular direction the size of each element was kept constant. The crack tip region was modelled using 36 semicircles. The ﬁrst of them was 25 times smaller than the last one. It also means that the ﬁrst ﬁnite element behind the crack tip was smaller 2000 times than the width of the specimen. The crack tip was modelled as a quarter of the arc whose radius was equal to

*rw* *= (1-2.5) · 10−6*m. Figure 4 presents exemplary ﬁnite element model for

CC(T) specimen.

Fig. 4. (a) The ﬁnite element model for CC(T) specimen used in the numerical analysis (due to the symmetry, only a quarter of the specimen was modelled);

(b) the crack tip model used for the CC(T) specimen

In the FEM simulation, the deformation theory of plasticity and the von Misses yield criterion were adopted. In the model, the stress-strain curve was approximated by the relation

*ε*
*ε*0
=
(
*σ/σ*0 for *σ ¬ σ*0
*α(σ/σ*0)*n* for *σ > σ*0
*where α = 1* (3.1)
The tensile properties for materials which were used in the numerical analysis
are presented below in Table 3. In the FEM analysis, calculations were done

for sixteen materials, which diﬀered by the yield stress and the work hardening exponent.

**Table 3. Mechanical properties of the materials used in numerical analysis**
*(σ*0 *– yield stress, E – Young’s modulusl ν – Poisson’s ratio, ε*0 – strain
*corre-sponding the yield stress, α – constant in the power law relationship, n work*
hardening exponent used in Eq. (3.1))

*σ*0 [MPa] *E [MPa]* *ν* *ε*0 *= σ*0*/E* *α* *n*
315
206000 0.3
0.00153
1
3
500 0.00243 5
1000 0.00485 10
1500 0.00728 20

*The J-integral was estimated using the “virtual shift method”. It uses the*
concept of virtual crack growth to compute virtual energy change (ADINA,
2006a,b).

In the numerical analysis, 64 CC(T) specimens were used, which diﬀered
*by the crack length (diﬀerent a/W ) and material properties (diﬀerent ratios*

*σ*0*/E and values of the power exponent n).*

**4.** **Numerical results – analysis of J-Q trajectories for CC(T)****specimens**

The analysis of the results obtained by the ﬁnite element method showed that
*in the range of distance from the crack tip J/σ*0 *< r < 6J/σ*0*, the Q-stress*
decreases if the distance from the crack tip increases (Fig. 5). If the external
*load increases, the Q-stress decreases and the diﬀerence between the Q-stress*
*calculated in the following measurement points (distance r from the crack tip)*
increases (Fig. 5).

*For the sake of the fact that the Q-parameter, which is used in the fracture*
*criterion, is calculated at a distance equal to r = 2J/σ*0 (which was proposed
by O’Dowd and Shih (1991, 1992)), it is necessary to carry out full analysis of
the obtained results at this distance from the crack tip.

*Assessing the inﬂuence of the crack length on the Q-stress value, it is*
*necessary to notice that if the crack length decreases, then the Q-stress *
*re-aches a greater negative value for the same J-integral level – see Fig. 6. For*
*CC(T) specimens characterised by a short crack, the J-Q curves reach faster*
the saturation level than for CC(T) specimens characterised by normative

*Fig. 5. “The J-Q family curves” for CC(T) specimen calculated at six distances r*
*for plane strain (W = 40 mm, a/W = 0.50, n = 10, ν = 0.3, E = 206000 MPa,*

*σ*0*= 1000 MPa, ε*0*= σ*0*/E = 0.001485); (a) whole loading spectrum, (b) magniﬁed*

portion of the graph

*Fig. 6. The inﬂuence of the crack length on the J-Q trajectories for CC(T) specimen*
*characterised by W = 40 mm, n = 10, ν = 0.3, E = 206000 MPa, σ*0= 1000 MPa,
*ε0= σ*0/E = 0.00485 (plane strain at the distance from the crack tip r = 2J/σ0)

*(a/W = 0.50) and long (a/W = 0.70) cracks. It may be noticed that for short*
*cracks, faster changes of the Q-parameter are observed if the external load*
increases (see the graphs in Appendices).

*As shown in Fig. 7, if the yield stress increases, the Q-parameter *
incre-ases too, and it reﬂects for all CC(T) specimens with diﬀerent crack lengths

*a/W . For smaller yield stresses, the J-Q trajectories shape up lower, and *

*(Fig. 7). Comparing the J-Q trajectories for diﬀerent values of σ0/E, it is *

ob-served that the biggest diﬀerences are characterised for materials with a small
*work-hardening exponent (n = 3 for strongly work-hardening materials) and*
the smallest for materials characterised by large work-hardening exponents
*(n = 20 for weakly work-hardening materials) – see the graphs in *
Appendi-ces. If the crack length increases, this diﬀerence somewhat increases too. For
*smaller yield stresses, the J-Q curves for CC(T) specimens reach the *
*satura-tion level for bigger external loads than the J-Q curves for CC(T) specimens*
characterised by large yield stresses.

*Fig. 7. The inﬂuence of the yield stress on J-Q (a) and Q = f (log[J/(aσ*0)]) (b)

*trajectories for CC(T): W = 40 mm, a/W = 0.50, n = 10, ν = 0.3, E = 206000 MPa*
*(plane strain for the distance from the crack tip r = 2J/σ*0)

*Figures 8 and 9 present some graphs of the J-Q trajectories which show the*
*inﬂuence of the work hardening exponent n on the Q-stress value and J-Q *
*cu-rves. If the yield stress decreases, the diﬀerences between the J-Q trajectories*
characterised for materials described by diﬀerent work-hardening exponents
*are bigger. For CC(T) specimens, ambiguous behaviour of the J-Q *
trajecto-ries depending of the work-hardening exponent is observed in comparison with
SEN(B) specimens, which was presented in Graba (2008). In most cases
*(dif-ferent relative crack lengths a/W , diﬀerent yield stresses (σ*0*/E 0.00364)),*
if the work-hardening exponent is smaller (strongly work-hardening
*mate-rials) than the Q-stress value increases (Fig. 9b). For small yield stresses*
*(0.00153 ¬ σ/E ¬ 0.00200), if the external load increases, then the Q-stress*

value decreases if the work-hardening exponent decreases (Fig. 8a). For
*mate-rials characterised by the yield stress σ*0*/E = 0.00243, the diﬀerence between*
*the J-Q trajectories are small. Mutual intersecting and overlapping of the*
trajectories are observed too (Fig. 9a).

*Fig. 8. The inﬂuence of the work-hardening exponent on J-Q (a) and*

*Q = f (log[J/(aσ0)]) (b) trajectories for CC(T): W = 40 mm, a/W = 0.20, ν = 0.3,*

*E = 206000 MPa, σ0= 315 MPa, ε*0*= σ*0/E = 0.00153 (plane strain for the distance

*from the crack tip r = 2J/σ*0)

*Fig. 9. The inﬂuence of the work-hardening exponent on J-Q trajectories for*
*CC(T): W = 40 mm, ν = 0.3, E = 206000 MPa and (a) a/W = 0.50, σ*0= 500 MPa,
*ε0= σ*0/E = 0.00243, (b) a/W = 0.70, σ0*= 1000 MPa, ε*0*= σ*0/E = 0.00485 (plane

*strain for the distance from the crack tip r = 2J/σ*0)

**5.** **Approximation of the numerical results for CC(T) specimens**

All the obtained in the numerical analysis results were used to create a
*catalo-gue of the J-Q trajectories for diﬀerent specimens (characterised by diﬀerent*
loading application, crack length) and diﬀerent materials. The presented in
the paper results are complementary with the directory presented in 2008 for
SEN(B) specimens (Graba, 2008). The current paper gives full numerical

re-sults for specimens with predominance of tension. The previous paper, which was mentioned above, gave numerical results and their approximation for spe-cimens with predominance of bending.

*The presented numerical computations provided the J-Q catalogue and*
*universal formula (5.1) which allows one to calculate the Q-stress for CC(T)*
specimens and take into consideration all the parameters inﬂuencing the value
*of the Q-stress. All results were presented in the Q = f (log[J/(aσ0)]) graph*
forms (for example see Fig. 8b and Fig. 10).

*Fig. 10. The inﬂuence of the work-hardening exponent on Q = f (log[J/(aσ*0)])

*trajectories for SEN(B) specimen: W = 40 mm, ν = 0.3, E = 206000 MPa,*
*(a) a/W = 0.50, σ*0*= 500 MPa, ε*0*= σ*0*/E = 0.00243 and (b) a/W = 0.70,*
*σ*0*= 1000 MPa, ε*0*= σ*0*/E = 0.00485; which were used in the procedure of*

approximation

Next, all graphs were approximated by simple mathematical formulas
ta-king the material properties, external load and geometry of the specimen into
consideration. All the approximations were made for the results obtained at
*the distance r = 2J/σ0. Each of the obtained trajectories Q = f (log[J/(aσ0)])*
was approximated by the third order polynomial in the form

*Q(J, a, σ*0*) = A + B log*
*J*
*aσ*0
*+ C*log *J*
*aσ*0
2
*+ D*log *J*
*aσ*0
3
(5.1)
*where the A, B, C, D coeﬃcients depend on the work-hardening exponent n,*
*yield stress σ*0 *and crack length a/W . The rank of the ﬁtting of formula*
*(5.1) to numerical results for the worst case was equal R*2 _{= 0.94 for the}*crack length a/W = 0.05. For other crack lengths a/W = {0.20, 0.50, 0.70},*
*the rank of the ﬁtting of formula (5.1) satisﬁed the condition R*2 * 0.99.*

*which were not included in the numerical analysis, the coeﬃcients A, B, C*
*and D may be evaluated using the linear or quadratic approximation. The*
results of numerical approximation using formula (5.1) for CC(T) specimens
(all coeﬃcients and the rank of the ﬁtting) are presented in Tables 4-7.
**Table 4. Coeﬃcients of equation (5.1) for CC(T) specimen with the crack**
*length a/W = 0.05*
*n* *A* *B* *C* *D* *R*2
*σ*0 *= 315 MPa, σ*0*/E = 0.00153*
3 *−1.79540* *−0.16046* 0.00270 *−0.05173* 0.979
5 *−1.84658* *−0.29915* *−0.12998* *−0.07354* 0.982
10 *−1.84196* *−0.61308* *−0.41668* *−0.13219* 0.961
20 *−1.74217* *−0.60418* *−0.44835* *−0.13965* 0.939
*σ*0 *= 1000 MPa, σ0/E = 0.00485*
3 *−1.54832* *−0.56730* *−0.33063* *−0.11413* 0.982
5 *−1.72656* *−0.63071* *−0.33882* *−0.10721* 0.986
10 *−1.49156* *−0.10931* *−0.03536* *−0.05032* 0.989
20 *−1.60795* *−0.40632* *−0.28062* *−0.10566* 0.996
*σ*0 *= 500 MPa, σ*0*/E = 0.00243*
3 *−1.61802* *−0.35121* *−0.26183* *−0.12290* 0.991
5 *−1.74621* *−0.47823* *−0.33828* *−0.12560* 0.980
10 *−1.79245* *−0.70894* *−0.52808* *−0.16144* 0.969
20 *−1.74847* *−0.77333* *−0.63058* *−0.18304* 0.934
*σ*0 *= 1500 MPa, σ*0*/E = 0.00728*
3 *−1.33418* *−0.24308* *−0.05234* *−0.04542* 0.951
5 *−1.51558* *−0.28024* *−0.05331* *−0.03969* 0.970
10 *−1.52391* *−0.19560* *−0.02477* *−0.03644* 0.981
20 *−1.59474* *−0.30780* *−0.10917* *−0.05471* 0.984

**Table 5. Coeﬃcients of equation (5.1) for CC(T) specimen with the crack**
*length a/W = 0.20*
*n* *A* *B* *C* *D* *R*2
*σ*0*= 315 MPa, σ*0*/E = 0.00153*
3 *−3.40016* *−2.97172* *−1.63678* *−0.33292* 0.995
5 *−2.81279* *−2.11444* *−1.22345* *−0.26738* 0.990
10 *−2.23934* *−1.40529* *−0.89907* *−0.21962* 0.999
20 *−2.13638* *−1.32808* *−0.84394* *−0.20595* 1.000

*σ*0*= 1000 MPa, σ*0*/E = 0.00485*
3 *−3.65130* *−3.39214* *−1.55538* *−0.26722* 0.973
5 *−1.67933* *−0.35103* *−0.11710* *−0.05261* 0.995
10 *−1.49619* *−0.12541* *−0.07218* *−0.05963* 0.997
20 *−1.53751* *−0.18282* *−0.11915* *−0.07285* 0.991
*σ*0 *= 500 MPa, σ0/E = 0.00243*
3 *−2.27413* *−1.18967* *−0.58590* *−0.13421* 0.992
5 *−2.29981* *−1.38659* *−0.81232* *−0.19438* 0.997
10 *−2.42665* *−1.88288* *−1.19659* *−0.27781* 0.998
20 *−2.57462* *−2.29845* *−1.48745* *−0.33839* 0.997
*σ*0*= 1500 MPa, σ*0*/E = 0.00728*
3 *−1.27982* 0.01996 0.14503 0.01481 0.989
5 *−1.41550* *−0.01120* 0.11191 *−0.00153* 0.994
10 *−1.54844* *−0.25319* *−0.11256* *−0.06390* 0.993
20 *−1.67907* *−0.45441* *−0.25880* *−0.10071* 0.994

**Table 6. Coeﬃcients of equation (5.1) for CC(T) specimen with the crack**
*length a/W = 0.50*
*n* *A* *B* *C* *D* *R*2
*σ*0*= 315 MPa, σ*0*/E = 0.00153*
3 *−3.85021* *−2.64950* *−1.05024* *−0.17336* 0.990
5 *−2.54684* *−1.13625* *−0.51015* *−0.11358* 0.997
10 *−2.24656* *−0.98456* *−0.50146* *−0.11605* 0.997
20 *−3.18413* *−2.55066* *−1.29798* *−0.24468* 0.996
*σ*0*= 1000 MPa, σ*0*/E = 0.00485*
3 *−3.42176* *−2.52110* *−0.90895* *−0.13071* 0.977
5 *−1.63674* 0.01781 0.19411 0.01940 0.994
10 *−1.68070* *−0.08345* 0.05407 *−0.02520* 0.997
20 *−1.88835* *−0.39917* *−0.13029* *−0.06196* 0.996
*σ*0*= 500 MPa, σ0/E = 0.00243*
3 *−3.55938* *−2.47891* *−0.95900* *−0.15488* 0.983
5 *−0.96124* 1.06111 0.56236 0.05471 0.998
10 *−1.61943* *−0.06732* *−0.04079* *−0.04818* 0.999
20 *−2.39669* *−1.42289* *−0.78360* *−0.17829* 0.999

*σ*0*= 1500 MPa, σ*0*/E = 0.00728*

3 *−1.27394* *−0.01699* 0.04887 *−0.01944* 0.997

5 *−1.57516* *−0.02788* 0.20193 0.03045 0.994

10 *−1.94130* *−0.43244* 0.01182 *−0.00341* 0.994

20 *−2.07357* *−0.56398* *−0.06157* *−0.02087* 0.995

**Table 7. Coeﬃcients of equation (5.1) for CC(T) specimen with the crack**
*length a/W = 0.70*
*n* *A* *B* *C* *D* *R*2
*σ*0*= 315 MPa, σ*0*/E = 0.00153*
3 *−3.39313* *−1.86453* *−0.70116* *−0.12257* 0.991
5 *−1.86720* *−0.11810* *−0.07379* *−0.05049* 0.998
10 *−3.70437* *−2.86445* *−1.35357* *−0.24114* 0.997
20 *−5.11211* *−4.87495* *−2.27736* *−0.37934* 0.997
*σ*0*= 1000 MPa, σ0/E = 0.00485*
3 *−2.93370* *−1.54934* *−0.40487* *−0.04995* 0.986
5 *−2.16067* *−0.26326* 0.17639 0.02853 0.997
10 *−2.42945* *−0.26930* 0.25072 0.04251 0.998
20 *−2.39733* *−0.11232* 0.32626 0.05005 0.998
*σ*0*= 500 MPa, σ*0*/E = 0.00243*
3 *−6.77352* *−5.84374* *−2.12683* *−0.28448* 0.981
5 *−2.14513* *−0.20561* 0.07296 *−0.00700* 0.997
10 *−2.09694* *−0.47913* *−0.18855* *−0.06352* 0.998
20 *−2.21086* *−0.88306* *−0.48750* *−0.12529* 0.999
*σ*0*= 1500 MPa, σ*0*/E = 0.00728*
3 *−2.02517* *−0.78494* *−0.17842* *−0.02840* 0.992
5 *−2.05092* *−0.46715* 0.02955 0.00524 0.989
10 *−2.10385* *−0.19800* 0.21559 0.03379 0.992
20 *−2.31937* *−0.32264* 0.19251 0.03093 0.996

Figure 11 presents the comparison of the numerical results and their
*ap-proximation for J-Q trajectories for several cases of the CC(T) specimens.*
Appendices A-D attached to the paper present in a graphical form (Figs.
12-15) all numerical results obtained for CC(T) specimens in plain strain. All
*results are presented using the J-Q trajectories for each analyzed case.*

*Fig. 11. Comparison of the numerical results and their approximation for J-Q*
*trajectories for CC(T) specimens: W = 40 mm, a/W = 0.50, E = 206000 MPa,*

*ν = 0.3 and (a) σ0∈ {315, 500} MPa, n ∈ {5, 10}, (b) σ0∈ {1000, 1500} MPa,*
*n ∈ {10, 20}*

**6.** **Conclusions**

*In the paper, values of the Q-stress were determined for various elastic-plastic*
materials for centrally cracked plate in tension (CC(T)). The inﬂuence of the
*yield strength, the work-hardening exponent and the crack length on the *
Q-parameter was tested. The numerical results were approximated by closed form
*formulas. In summary, it may be concluded that the Q-stress depends on *
*geo-metry and the external load. Diﬀerent values of the Q-stress are obtained for*
a centrally cracked plane in tension (CC(T)) and diﬀerent for the SEN(B)
specimen, which was characterised by the same material properties (see
*Ap-pendices of this paper and ApAp-pendices in Graba (2008)). The Q-parameter is*
a function of the material properties; its value depends on the work-hardening
*exponent n and the yield stress σ*0*. If the crack length decreases, then Q-stress*
reaches greater negative value for the same external load.

*The presented in the paper catalogue of the Q-stress values and J-Q*
trajectories for specimens with predominance of tension (CC(T) specimens) is
complementary with the numerical solution presented in Graba (2008), which
*gave J-Q trajectories for specimens with predominance of bending (SEN(B)*
specimens)). Both papers may be quite useful for solving engineering problems
in which the fracture toughness or stress distribution near the crack tip must
be quite fast estimated.

**Appendix A. Numerical results for CC(T) specimen in plane strain**
**with the crack length a/W = 0.05 (distance from the crack tip**

*r = 2J/σ*0**)**

*Fig. 12. The inﬂuence of the yield stress on J-Q trajectories for CC(T) specimens*
*with the crack length a/W = 0.05 for diﬀerent power exponents in R-O*
*relationship: (a) n = 3, (b) n = 5, (c) n = 10, (d) n = 20 (W = 40 mm, ν = 0.3,*

**Appendix B. Numerical results for CC(T) specimen in plane strain**
**with the crack length a/W = 0.20 (distance from the crack tip**

*r = 2J/σ*0**)**

*Fig. 13. The inﬂuence of the yield stress on J-Q trajectories for CC(T) specimens*
*with the crack length a/W = 0.20 for diﬀerent power exponents in R-O*
*relationship: (a) n = 3, (b) n = 5, (c) n = 10, (d) n = 20 (W = 40 mm, ν = 0.3,*

**Appendix C. Numerical results for CC(T) specimen in plane strain**
**with the crack length a/W = 0.50 (distance from the crack tip**

*r = 2.J/σ*0**)**

*Fig. 14. The inﬂuence of the yield stress on J-Q trajectories for CC(T) specimens*
*with the crack length a/W = 0.50 for diﬀerent power exponents in R-O*
*relationship: (a) n = 3, (b) n = 5, (c) n = 10, (d) n = 20 (W = 40 mm, ν = 0.3,*

**Appendix D. Numerical results for CC(T) specimen in plane**
**strain with the crack length a/W = 0.70 (distance from the crack**

* tip r = 2J/σ*0

**)**

*Fig. 15. The inﬂuence of the yield stress on J-Q trajectories for CC(T) specimens*
*with the crack length a/W = 0.70 for diﬀerent power exponents in R-O*
*relationship: (a) n = 3, (b) n = 5, (c) n = 10, (d) n = 20 (W = 40 mm, ν = 0.3,*

*E = 206000 MPa)*

*Acknowledgements*

The support of Kielce University of Technology, Faculty of Mechatronics and Machine Design through grant No. 1.22/8.57 is acknowledged by the author of the paper.

**References**

1. ADINA 2006a, ADINA 8.4.1: User Interface Command Reference Manual – Volume I: ADINA Solids & Structures Model Deﬁnition, Report ARD 06-2, ADINA R&D, Inc.

2. ADINA 2006b, ADINA 8.4.1: Theory and Modeling Guide – Volume I: ADINA, Report ARD 06-7, ADINA R&D, Inc.

3. Ainsworth R.A., O’Dowd N.P., 1994, A framework of including constra-int eﬀects in the failure assessment diagram approach for fracture assessment,

*ASME Pressure Vessels and Piping Conference, ASME, PVP-Vol *

287/MD-Vol 47

4. FITNET, 2006, FITNET Report, (European Fitness-for-service Network), Edi-ted by M. Kocak, S. Webster, J.J. Janosch, R.A. Ainsworth, R. Koers, Contract No. G1RT-CT-2001-05071

5. Gałkiewicz J., Graba M., 2006, Algorithm for determination of e*σij(n, θ),*

e

*εij(n, θ), eui(n, θ), dn(n), and In(n) functions in Hutchinson-Rice-Rosengren *

*so-lution and its 3D generalization, Journal of Theoretical and Applied Mechanics,*
**44, 1, 19-30**

*6. Graba M., 2008, The inﬂuence of material properties on the Q-stress value *
*ne-ar the crack tip for elastic-plastic materials, Journal of Theoretical and Applied*

**Mechanics, 46, 2, 269-290**

7. Hutchinson J.W., 1968, Singular behaviour at the end of a tensile crack in a
* hardening material, Journal of the Mechanics and Physics of Solids, 16, 13-31*
8. Kumar V., German M.D., Shih C.F., 1981, An engineering approach for

*elastic-plastic fracture analysis, EPRI Report NP-1931, Electric Power Research*Institute, Palo Alto, CA

9. Li Y., Wang Z., 1985, High-order asymptotic ﬁeld of tensile plane-strain
**non-linear crack problems, Scientia Sinica (Series A), XXIX, 9, 941-955**

10. Neimitz A., Dzioba I., Molasy R., Graba M., 2004, Wpływ więzów na
*od-porność na pękanie materiałów kruchych, Materiały XX Sympozjum Zmęczenia*

*i Mechaniki Pękania, Bydgoszcz-Pieczyska, 265-272*

11. Neimitz A., Graba M., Gałkiewicz J., 2007, An alternative formulation
*of the Ritchie-Knott-Rice local fracture criterion, Engineering Fracture *

**Mecha-nics, 74, 1308-1322**

12. O’Dowd N.P., 1995, Applications of two parameter approaches in
* elastic-plastic fracture mechanics, Engineering Fracture Mechanics, 52, 3, 445-465*
13. O’Dowd N.P., Shih C.F., 1991, Family of crack-tip ﬁelds characterized by

* a triaxiality parameter – I. Structure of ﬁelds, J. Mech. Phys. Solids, 39, 8,*
989-1015

14. O’Dowd N.P., Shih C.F., 1992, Family of crack-tip ﬁelds characterized by a
* triaxiality parameter – II. Fracture applications, J. Mech. Phys. Solids, 40, 5,*
939-963

15. Ritchie R.O., Knott J.F., Rice J.R., 1973, On the relationship
*betwe-en critical tbetwe-ensile stress and fracture toughness in mild steel, Journal of the*

**Mechanics and Physics of Solids, 21, 395-410**

16. SINTAP, 1999, SINTAP: Structural Integrity Assessment Procedures for Eu-ropean Industry. Final Procedure, Brite-Euram Project No. BE95-1426 – Ro-therham: British Steel

17. Sherry, A.H., Wilkes M.A., Beardsmore D.W., Lidbury D.P.G.,
2005a, Material constraint parameters for the assessment of shallow defects
*in structural componenets – Part I: Parameter solutions, Engineering Fracture*

**Mechanics, 72, 2373-2395**

18. Sherry A.H., Hooton D.G., Beardsmore D.W., Lidbury D.P.G., 2005b, Material constraint parameters for the assessment of shallow defects in struc-tural components – Part II: Constraint – based assessment of shallow cracks,

**Engineering Fracture Mechanics, 72, 2396-2415**

19. Shih C.F., O’Dowd N.P., Kirk M.T., 1993, A framework for quantifying
*crack tip constraint, [In:] Constraint Eﬀects in Fracture, ASTM STP 1171, E.M.*
Hackett, K,-H. Schwalbe, R.H. Dodds, Eds., American Society for Testing and
Materials, Philadelphia, 2-20

20. Sumpter J.D.G., Forbes A.T., 1992, Constraint based analysis of shallow
*cracks in mild steel, TWI/EWI/IS International Conference on Shallow Crack*

*Fracture Mechanics Test and Application, M.G. Dawes, Edit., Cambridge, UK,*

paper 7

21. Yang S., Chao Y.J., Sutton M.A., 1993, Higher order asymptotic crack
* tip in a power-law hardening material, Engineering Fracture Mechanics, 45, 1,*
99-120

**Wpływ stałych materiałowych i długości pęknięcia na rozkład**
**naprężeń Q przed wierzchołkiem pęknięcia w materiałach****sprężysto-plastycznych dla płyty z centralną szczeliną poddanej**

**rozciąganiu**
Streszczenie

*W pracy przedstawione zostały wartości naprężeń Q wyznaczone dla szeregu *
ma-teriałów sprężysto-plastycznych dla płyt z centralną szczeliną na wskroś
poddawa-nych rozciąganiu (CC(T)). Omówiony został wpływ granicy plastyczności i
*wykład-nika umocnienia na wartość naprężeń Q, a także wpływ długości pęknięcia. Wyniki*

obliczeń numerycznych aproksymowano formułami analitycznymi. Rezultaty pracy
*stanowią podręczny katalog krzywych J-Q dla próbek CC(T) – próbek z przewagą*
rozciągania, możliwy do wykorzystania w praktyce inżynierskiej. Prezentowane wyniki
są kontynuacją katalogu zaprezentowanego w roku 2008], który zawierał
numerycz-ne rozwiązania i ich aproksymacje dla próbek z przewagą zginania (próbki SEN(B)).
Oba elementy konstrukcyjne (próbki CC(T) i SEN(B)) często są wykorzystywane
do wyznaczania odporności na pękanie w warunkach laboratoryjnych, a w analizie
inżynierskiej stosuje się je jako uproszczenie złożonego obiektu konstrukcyjnego, co
zalecane jest w procedurach FITNET.